#------------------------------------------------------------------------------
#$Date: 2016-03-23 21:03:00 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179437 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/34/4333403.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_4333403
loop_
_publ_author_name
'Alekseev, Evgeny V.'
'Krivovichev, Sergey V.'
'Malcherek, Thomas'
'Depmeier, Wulf'
_publ_section_title
;
 One-Dimensional Array of Two- and Three-Center Cation−Cation Bonds
 in the Structure of Li4[(UO2)10O10(Mo2O8)]
;
_journal_issue                   21
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              8442
_journal_page_last               8444
_journal_paper_doi               10.1021/ic7009385
_journal_volume                  46
_journal_year                    2007
_chemical_formula_moiety         Li4U10Mo2O38
_chemical_formula_sum            'Li4 Mo2 O38 U10'
_chemical_formula_weight         3207.94
_chemical_melting_point          ?
_chemical_name_common            'lithium uranyl molybdate'
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.575(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   7.9426(4)
_cell_length_b                   19.9895(9)
_cell_length_c                   10.0796(5)
_cell_measurement_reflns_used    877
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      23.44
_cell_measurement_theta_min      3.62
_cell_volume                     1600.24(13)
_computing_cell_refinement       DENZO
_computing_data_collection       'Nonius Kappa CCD'
_computing_data_reduction        DENZO
_computing_molecular_graphics    'Atoms 6.1'
_computing_publication_material  Wingx
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 0.2
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Nonius Kappa CCD'
_diffrn_measurement_method       phi-scan
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0952
_diffrn_reflns_av_sigmaI/netI    0.0460
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       24
_diffrn_reflns_limit_k_min       -24
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            17972
_diffrn_reflns_theta_full        26.36
_diffrn_reflns_theta_max         26.36
_diffrn_reflns_theta_min         2.02
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count 100
_diffrn_standards_interval_time  10
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    51.273
_exptl_absorpt_correction_T_max  0.4953
_exptl_absorpt_correction_T_min  0.0602
_exptl_absorpt_correction_type   analytical
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    6.658
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             2640
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.16
_exptl_crystal_size_min          0.07
_refine_diff_density_max         6.492
_refine_diff_density_min         -5.159
_refine_diff_density_rms         1.675
_refine_ls_extinction_coef       0.00043(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   0.936
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     249
_refine_ls_number_reflns         3265
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.936
_refine_ls_R_factor_all          0.0494
_refine_ls_R_factor_gt           0.0429
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0732P)²+151.0427P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1166
_refine_ls_wR_factor_ref         0.1210
_reflns_number_gt                3134
_reflns_number_total             3265
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic7009385sup1.cif
_cod_data_source_block           output
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' value 'unknown' was changed to '?' - the
value is undefined or not given.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_database_code               4333403
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
U1 U 0.22933(11) 0.73601(3) 0.94060(7) 0.0145(2) Uani 1 1 d .
U2 U -0.02551(11) 0.63888(4) 1.18496(8) 0.0125(2) Uani 1 1 d .
U3 U 0.48332(11) 0.63627(4) 1.18236(8) 0.0129(2) Uani 1 1 d .
U4 U 0.72527(11) 0.75313(3) 0.90703(7) 0.0146(2) Uani 1 1 d .
U5 U 0.5000 0.5000 0.5000 0.0143(3) Uani 1 2 d S
U6 U 0.0000 0.5000 0.5000 0.0147(3) Uani 1 2 d S
Mo Mo -0.2094(3) 0.51016(9) 0.97000(19) 0.0196(4) Uani 1 1 d .
O1 O -0.277(2) 0.5690(8) 1.0963(17) 0.031(4) Uani 1 1 d .
O2 O -0.370(2) 0.4507(8) 0.9605(18) 0.026(4) Uani 1 1 d .
O3 O -0.033(2) 0.4440(7) 0.9619(18) 0.023(4) Uani 1 1 d .
O4 O 0.453(2) 0.5747(8) 1.3182(15) 0.019(3) Uani 1 1 d .
O5 O 0.021(2) 0.5764(8) 1.3197(17) 0.021(4) Uani 1 1 d .
O6 O 0.063(2) 0.5665(9) 0.6191(17) 0.025(4) Uani 1 1 d .
O7 O 0.008(2) 0.7185(8) 1.3275(15) 0.018(3) Uani 1 1 d .
O8 O 0.728(2) 0.8197(7) 1.0268(15) 0.021(3) Uani 1 1 d .
O9 O 0.448(2) 0.7162(8) 1.3322(16) 0.025(4) Uani 1 1 d .
O10 O 0.227(2) 0.6636(7) 1.1328(14) 0.022(3) Uani 1 1 d .
O11 O 0.225(2) 0.6624(7) 0.8357(15) 0.023(3) Uani 1 1 d .
O12 O 0.234(2) 0.8051(7) 1.0536(15) 0.022(3) Uani 1 1 d .
O13 O 0.511(2) 0.6960(8) 1.0340(15) 0.018(3) Uani 1 1 d .
O14 O 0.2519(18) 0.4677(7) 0.4776(14) 0.017(3) Uani 1 1 d .
O15 O 0.446(2) 0.5659(7) 0.6176(17) 0.021(3) Uani 1 1 d .
O16 O -0.269(2) 0.6678(7) 1.2495(15) 0.021(3) Uani 1 1 d .
O17 O -0.222(3) 0.5490(8) 0.8177(15) 0.031(4) Uani 1 1 d .
O18 O -0.060(2) 0.6984(8) 1.0352(17) 0.021(3) Uani 1 1 d .
O19 O 0.720(2) 0.6851(7) 0.7930(15) 0.026(4) Uani 1 1 d .
Li1 Li 0.255(6) 0.6172(18) 0.673(5) 0.036(11) Uani 1 1 d .
Li2 Li -0.275(8) 0.606(2) 0.660(5) 0.045(13) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
U U -9.6767 9.6646 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O12 U1 O11 176.2(7) . .
O12 U1 O9 88.3(7) . 4_575
O11 U1 O9 94.0(7) . 4_575
O12 U1 O7 91.2(7) . 4_575
O11 U1 O7 91.4(7) . 4_575
O9 U1 O7 100.4(6) 4_575 4_575
O12 U1 O10 87.3(6) . .
O11 U1 O10 88.9(6) . .
O9 U1 O10 130.6(6) 4_575 .
O7 U1 O10 128.9(6) 4_575 .
O12 U1 O13 89.7(6) . .
O11 U1 O13 88.3(6) . .
O9 U1 O13 68.7(6) 4_575 .
O7 U1 O13 169.0(5) 4_575 .
O10 U1 O13 62.1(5) . .
O12 U1 O18 90.1(7) . .
O11 U1 O18 88.3(6) . .
O9 U1 O18 167.8(5) 4_575 .
O7 U1 O18 67.6(5) 4_575 .
O10 U1 O18 61.3(5) . .
O13 U1 O18 123.3(5) . .
O12 U1 Li1 169.8(9) . .
O11 U1 Li1 13.6(9) . .
O9 U1 Li1 82.4(9) 4_575 .
O7 U1 Li1 86.4(8) 4_575 .
O10 U1 Li1 101.9(8) . .
O13 U1 Li1 90.7(8) . .
O18 U1 Li1 98.1(9) . .
O12 U1 U3 89.4(5) . .
O11 U1 U3 87.3(5) . .
O9 U1 U3 97.4(4) 4_575 .
O7 U1 U3 162.2(4) 4_575 .
O10 U1 U3 33.4(4) . .
O13 U1 U3 28.7(4) . .
O18 U1 U3 94.6(3) . .
Li1 U1 U3 95.9(7) . .
O12 U1 U2 89.4(5) . .
O11 U1 U2 87.5(5) . .
O9 U1 U2 162.8(4) 4_575 .
O7 U1 U2 96.7(4) 4_575 .
O10 U1 U2 32.2(4) . .
O13 U1 U2 94.2(4) . .
O18 U1 U2 29.1(3) . .
Li1 U1 U2 100.7(8) . .
U3 U1 U2 65.50(2) . .
O12 U1 Li1 2.2(9) . 4_576
O11 U1 Li1 176.4(9) . 4_576
O9 U1 Li1 86.2(9) 4_575 4_576
O7 U1 Li1 92.2(8) 4_575 4_576
O10 U1 Li1 88.2(8) . 4_576
O13 U1 Li1 88.4(8) . 4_576
O18 U1 Li1 92.3(8) . 4_576
Li1 U1 Li1 168.0(14) . 4_576
U3 U1 Li1 89.1(7) . 4_576
U2 U1 Li1 91.2(7) . 4_576
O12 U1 U4 88.5(6) . .
O11 U1 U4 91.8(5) . .
O9 U1 U4 32.8(4) 4_575 .
O7 U1 U4 133.2(4) 4_575 .
O10 U1 U4 97.9(4) . .
O13 U1 U4 35.9(3) . .
O18 U1 U4 159.2(3) . .
Li1 U1 U4 85.9(8) . .
U3 U1 U4 64.59(2) . .
U2 U1 U4 130.06(3) . .
Li1 U1 U4 86.4(7) 4_576 .
O5 U2 O18 174.7(7) . .
O5 U2 O16 97.6(7) . .
O18 U2 O16 87.0(6) . .
O5 U2 O10 98.9(6) . .
O18 U2 O10 78.0(6) . .
O16 U2 O10 150.6(6) . .
O5 U2 O7 89.3(7) . .
O18 U2 O7 94.6(7) . .
O16 U2 O7 72.7(6) . .
O10 U2 O7 83.3(6) . .
O5 U2 O3 86.9(7) . 3_567
O18 U2 O3 88.2(6) . 3_567
O16 U2 O3 126.0(6) . 3_567
O10 U2 O3 79.1(6) . 3_567
O7 U2 O3 161.2(6) . 3_567
O5 U2 O1 92.1(6) . .
O18 U2 O1 87.7(6) . .
O16 U2 O1 63.3(6) . .
O10 U2 O1 139.7(6) . .
O7 U2 O1 135.8(6) . .
O3 U2 O1 62.8(6) 3_567 .
O5 U2 Mo 92.0(5) . .
O18 U2 Mo 85.3(5) . .
O16 U2 Mo 90.8(4) . .
O10 U2 Mo 112.8(4) . .
O7 U2 Mo 163.5(4) . .
O3 U2 Mo 35.3(4) 3_567 .
O1 U2 Mo 27.7(4) . .
O5 U2 U4 93.0(5) . 4_476
O18 U2 U4 92.3(5) . 4_476
O16 U2 U4 33.1(4) . 4_476
O10 U2 U4 121.6(4) . 4_476
O7 U2 U4 39.7(4) . 4_476
O3 U2 U4 158.9(4) 3_567 4_476
O1 U2 U4 96.2(4) . 4_476
Mo U2 U4 123.79(4) . 4_476
O5 U2 U1 135.8(5) . .
O18 U2 U1 40.9(5) . .
O16 U2 U1 124.0(4) . .
O10 U2 U1 37.2(4) . .
O7 U2 U1 89.5(4) . .
O3 U2 U1 80.5(4) 3_567 .
O1 U2 U1 118.2(4) . .
Mo U2 U1 100.96(4) . .
U4 U2 U1 113.04(2) 4_476 .
O5 U2 U3 100.7(5) . 1_455
O18 U2 U3 82.4(5) . 1_455
O16 U2 U3 24.9(4) . 1_455
O10 U2 U3 160.4(4) . 1_455
O7 U2 U3 97.6(4) . 1_455
O3 U2 U3 101.3(4) 3_567 1_455
O1 U2 U3 39.0(4) . 1_455
Mo U2 U3 66.01(4) . 1_455
U4 U2 U3 58.04(2) 4_476 1_455
U1 U2 U3 123.32(3) . 1_455
O5 U2 U3 78.9(5) . .
O18 U2 U3 97.9(5) . .
O16 U2 U3 156.6(4) . .
O10 U2 U3 20.0(4) . .
O7 U2 U3 84.1(4) . .
O3 U2 U3 77.1(4) 3_567 .
O1 U2 U3 139.4(4) . .
Mo U2 U3 112.35(4) . .
U4 U2 U3 123.55(3) 4_476 .
U1 U2 U3 57.014(19) . .
U3 U2 U3 178.32(3) 1_455 .
O4 U3 O13 176.6(7) . .
O4 U3 O10 102.0(7) . .
O13 U3 O10 77.3(6) . .
O4 U3 O16 95.0(7) . 1_655
O13 U3 O16 87.1(6) . 1_655
O10 U3 O16 148.1(5) . 1_655
O4 U3 O9 87.5(7) . .
O13 U3 O9 95.7(6) . .
O10 U3 O9 81.3(6) . .
O16 U3 O9 72.5(6) 1_655 .
O4 U3 O2 85.0(7) . 3_567
O13 U3 O2 91.6(6) . 3_567
O10 U3 O2 72.6(6) . 3_567
O16 U3 O2 136.4(5) 1_655 3_567
O9 U3 O2 150.6(6) . 3_567
O4 U3 O1 90.3(6) . 1_655
O13 U3 O1 88.2(6) . 1_655
O10 U3 O1 140.9(5) . 1_655
O16 U3 O1 64.7(5) 1_655 1_655
O9 U3 O1 136.8(6) . 1_655
O2 U3 O1 71.8(5) 3_567 1_655
O4 U3 U4 90.9(5) . 4_576
O13 U3 U4 92.4(4) . 4_576
O10 U3 U4 118.3(4) . 4_576
O16 U3 U4 33.8(4) 1_655 4_576
O9 U3 U4 38.8(5) . 4_576
O2 U3 U4 169.1(4) 3_567 4_576
O1 U3 U4 98.2(4) 1_655 4_576
O4 U3 U1 139.7(5) . .
O13 U3 U1 39.4(5) . .
O10 U3 U1 37.9(4) . .
O16 U3 U1 122.2(4) 1_655 .
O9 U3 U1 89.3(4) . .
O2 U3 U1 78.4(4) 3_567 .
O1 U3 U1 118.1(4) 1_655 .
U4 U3 U1 110.85(2) 4_576 .
O4 U3 U2 98.2(5) . 1_655
O13 U3 U2 82.7(5) . 1_655
O10 U3 U2 159.7(4) . 1_655
O16 U3 U2 24.4(4) 1_655 1_655
O9 U3 U2 96.9(5) . 1_655
O2 U3 U2 112.3(4) 3_567 1_655
O1 U3 U2 40.8(4) 1_655 1_655
U4 U3 U2 58.22(2) 4_576 1_655
U1 U3 U2 122.14(3) . 1_655
O4 U3 U2 82.3(5) . .
O13 U3 U2 96.9(5) . .
O10 U3 U2 19.7(4) . .
O16 U3 U2 154.0(4) 1_655 .
O9 U3 U2 81.5(5) . .
O2 U3 U2 69.4(4) 3_567 .
O1 U3 U2 140.9(4) 1_655 .
U4 U3 U2 120.18(3) 4_576 .
U1 U3 U2 57.49(2) . .
U2 U3 U2 178.32(3) 1_655 .
O19 U4 O8 177.9(7) . .
O19 U4 O16 94.7(6) . 4_675
O8 U4 O16 87.3(6) . 4_675
O19 U4 O18 90.7(7) . 1_655
O8 U4 O18 88.3(7) . 1_655
O16 U4 O18 133.3(6) 4_675 1_655
O19 U4 O9 88.6(7) . 4_575
O8 U4 O9 91.6(7) . 4_575
O16 U4 O9 67.8(6) 4_675 4_575
O18 U4 O9 158.8(5) 1_655 4_575
O19 U4 O13 88.2(7) . .
O8 U4 O13 89.9(6) . .
O16 U4 O13 136.5(6) 4_675 .
O18 U4 O13 89.9(5) 1_655 .
O9 U4 O13 68.9(6) 4_575 .
O19 U4 O7 89.0(7) . 4_675
O8 U4 O7 92.4(6) . 4_675
O16 U4 O7 65.3(5) 4_675 4_675
O18 U4 O7 68.5(5) 1_655 4_675
O9 U4 O7 132.7(5) 4_575 4_675
O13 U4 O7 158.2(5) . 4_675
O19 U4 U3 93.0(5) . 4_575
O8 U4 U3 88.4(5) . 4_575
O16 U4 U3 32.5(4) 4_675 4_575
O18 U4 U3 165.6(4) 1_655 4_575
O9 U4 U3 35.3(4) 4_575 4_575
O13 U4 U3 104.1(4) . 4_575
O7 U4 U3 97.7(4) 4_675 4_575
O19 U4 U2 93.7(6) . 4_675
O8 U4 U2 88.3(5) . 4_675
O16 U4 U2 31.2(4) 4_675 4_675
O18 U4 U2 102.2(4) 1_655 4_675
O9 U4 U2 99.0(4) 4_575 4_675
O13 U4 U2 167.7(4) . 4_675
O7 U4 U2 34.1(4) 4_675 4_675
U3 U4 U2 63.74(2) 4_575 4_675
O19 U4 Li2 177.6(11) . 4_676
O8 U4 Li2 0.8(11) . 4_676
O16 U4 Li2 87.2(9) 4_675 4_676
O18 U4 Li2 89.0(9) 1_655 4_676
O9 U4 Li2 90.8(10) 4_575 4_676
O13 U4 Li2 89.5(10) . 4_676
O7 U4 Li2 93.1(11) 4_675 4_676
U3 U4 Li2 87.8(7) 4_575 4_676
U2 U4 Li2 88.6(9) 4_675 4_676
O19 U4 U1 88.3(6) . .
O8 U4 U1 90.8(5) . .
O16 U4 U1 98.5(4) 4_675 .
O18 U4 U1 128.0(4) 1_655 .
O9 U4 U1 30.8(4) 4_575 .
O13 U4 U1 38.1(4) . .
O7 U4 U1 163.3(4) 4_675 .
U3 U4 U1 65.99(2) 4_575 .
U2 U4 U1 129.73(3) 4_675 .
Li2 U4 U1 90.0(10) 4_676 .
O19 U4 U1 90.4(6) . 1_655
O8 U4 U1 90.0(5) . 1_655
O16 U4 U1 95.3(4) 4_675 1_655
O18 U4 U1 38.2(4) 1_655 1_655
O9 U4 U1 162.9(4) 4_575 1_655
O13 U4 U1 128.1(4) . 1_655
O7 U4 U1 30.3(4) 4_675 1_655
U3 U4 U1 127.83(3) 4_575 1_655
U2 U4 U1 64.09(2) 4_675 1_655
Li2 U4 U1 90.8(10) 4_676 1_655
U1 U4 U1 166.18(3) . 1_655
O15 U5 O15 180.0(10) . 3_666
O15 U5 O14 86.1(6) . 3_666
O15 U5 O14 93.9(6) 3_666 3_666
O15 U5 O14 93.9(6) . .
O15 U5 O14 86.1(6) 3_666 .
O14 U5 O14 180.0(7) 3_666 .
O15 U5 O4 90.7(6) . 1_554
O15 U5 O4 89.3(6) 3_666 1_554
O14 U5 O4 91.8(6) 3_666 1_554
O14 U5 O4 88.2(6) . 1_554
O15 U5 O4 89.3(6) . 3_667
O15 U5 O4 90.7(6) 3_666 3_667
O14 U5 O4 88.2(6) 3_666 3_667
O14 U5 O4 91.8(6) . 3_667
O4 U5 O4 180.0(6) 1_554 3_667
O15 U5 Li2 47.8(13) . 1_655
O15 U5 Li2 132.2(13) 3_666 1_655
O14 U5 Li2 38.4(12) 3_666 1_655
O14 U5 Li2 141.6(12) . 1_655
O4 U5 Li2 93.2(8) 1_554 1_655
O4 U5 Li2 86.8(8) 3_667 1_655
O15 U5 Li2 132.2(13) . 3_566
O15 U5 Li2 47.8(13) 3_666 3_566
O14 U5 Li2 141.6(12) 3_666 3_566
O14 U5 Li2 38.4(12) . 3_566
O4 U5 Li2 86.8(8) 1_554 3_566
O4 U5 Li2 93.2(8) 3_667 3_566
Li2 U5 Li2 180.000(5) 1_655 3_566
O15 U5 Li1 20.6(9) . .
O15 U5 Li1 159.4(9) 3_666 .
O14 U5 Li1 105.5(8) 3_666 .
O14 U5 Li1 74.5(8) . .
O4 U5 Li1 83.2(9) 1_554 .
O4 U5 Li1 96.8(9) 3_667 .
Li2 U5 Li1 67.6(13) 1_655 .
Li2 U5 Li1 112.4(13) 3_566 .
O15 U5 Li1 159.4(10) . 3_666
O15 U5 Li1 20.6(9) 3_666 3_666
O14 U5 Li1 74.5(8) 3_666 3_666
O14 U5 Li1 105.5(8) . 3_666
O4 U5 Li1 96.8(9) 1_554 3_666
O4 U5 Li1 83.2(9) 3_667 3_666
Li2 U5 Li1 112.4(13) 1_655 3_666
Li2 U5 Li1 67.6(13) 3_566 3_666
Li1 U5 Li1 180.000(4) . 3_666
O15 U5 U6 76.1(5) . .
O15 U5 U6 103.9(5) 3_666 .
O14 U5 U6 160.8(4) 3_666 .
O14 U5 U6 19.2(4) . .
O4 U5 U6 81.4(4) 1_554 .
O4 U5 U6 98.6(4) 3_667 .
Li2 U5 U6 123.7(12) 1_655 .
Li2 U5 U6 56.3(12) 3_566 .
Li1 U5 U6 56.1(8) . .
Li1 U5 U6 123.9(8) 3_666 .
O15 U5 U6 103.9(5) . 1_655
O15 U5 U6 76.1(5) 3_666 1_655
O14 U5 U6 19.2(4) 3_666 1_655
O14 U5 U6 160.8(4) . 1_655
O4 U5 U6 98.6(4) 1_554 1_655
O4 U5 U6 81.4(4) 3_667 1_655
Li2 U5 U6 56.3(12) 1_655 1_655
Li2 U5 U6 123.7(12) 3_566 1_655
Li1 U5 U6 123.9(8) . 1_655
Li1 U5 U6 56.1(8) 3_666 1_655
U6 U5 U6 180.0 . 1_655
O6 U6 O6 180.0(8) . 3_566
O6 U6 O14 87.7(6) . 3_566
O6 U6 O14 92.3(6) 3_566 3_566
O6 U6 O14 92.3(6) . .
O6 U6 O14 87.7(6) 3_566 .
O14 U6 O14 180.000(2) 3_566 .
O6 U6 O5 89.2(7) . 3_567
O6 U6 O5 90.8(7) 3_566 3_567
O14 U6 O5 92.3(5) 3_566 3_567
O14 U6 O5 87.7(5) . 3_567
O6 U6 O5 90.8(7) . 1_554
O6 U6 O5 89.2(7) 3_566 1_554
O14 U6 O5 87.7(5) 3_566 1_554
O14 U6 O5 92.3(5) . 1_554
O5 U6 O5 180.0(6) 3_567 1_554
O6 U6 Li2 55.0(10) . .
O6 U6 Li2 125.0(11) 3_566 .
O14 U6 Li2 32.8(10) 3_566 .
O14 U6 Li2 147.2(10) . .
O5 U6 Li2 89.3(8) 3_567 .
O5 U6 Li2 90.7(8) 1_554 .
O6 U6 Li2 125.0(11) . 3_566
O6 U6 Li2 55.0(10) 3_566 3_566
O14 U6 Li2 147.2(10) 3_566 3_566
O14 U6 Li2 32.8(10) . 3_566
O5 U6 Li2 90.7(8) 3_567 3_566
O5 U6 Li2 89.3(8) 1_554 3_566
Li2 U6 Li2 180.000(5) . 3_566
O6 U6 Li1 20.0(10) . .
O6 U6 Li1 160.0(10) 3_566 .
O14 U6 Li1 106.4(8) 3_566 .
O14 U6 Li1 73.6(8) . .
O5 U6 Li1 95.3(9) 3_567 .
O5 U6 Li1 84.7(9) 1_554 .
Li2 U6 Li1 74.2(11) . .
Li2 U6 Li1 105.8(11) 3_566 .
O6 U6 Li1 160.0(10) . 3_566
O6 U6 Li1 20.0(10) 3_566 3_566
O14 U6 Li1 73.6(8) 3_566 3_566
O14 U6 Li1 106.4(8) . 3_566
O5 U6 Li1 84.7(9) 3_567 3_566
O5 U6 Li1 95.3(9) 1_554 3_566
Li2 U6 Li1 105.8(11) . 3_566
Li2 U6 Li1 74.2(11) 3_566 3_566
Li1 U6 Li1 180.000(3) . 3_566
O6 U6 U5 105.1(5) . 1_455
O6 U6 U5 74.9(5) 3_566 1_455
O14 U6 U5 18.8(4) 3_566 1_455
O14 U6 U5 161.2(4) . 1_455
O5 U6 U5 85.6(4) 3_567 1_455
O5 U6 U5 94.4(4) 1_554 1_455
Li2 U6 U5 50.3(9) . 1_455
Li2 U6 U5 129.7(9) 3_566 1_455
Li1 U6 U5 124.6(7) . 1_455
Li1 U6 U5 55.4(7) 3_566 1_455
O6 U6 U5 74.9(5) . .
O6 U6 U5 105.1(5) 3_566 .
O14 U6 U5 161.2(4) 3_566 .
O14 U6 U5 18.8(4) . .
O5 U6 U5 94.4(4) 3_567 .
O5 U6 U5 85.6(4) 1_554 .
Li2 U6 U5 129.7(9) . .
Li2 U6 U5 50.3(9) 3_566 .
Li1 U6 U5 55.4(7) . .
Li1 U6 U5 124.6(7) 3_566 .
U5 U6 U5 180.0 1_455 .
O17 Mo O2 102.8(9) . .
O17 Mo O1 108.5(8) . .
O2 Mo O1 104.9(8) . .
O17 Mo O3 107.9(8) . .
O2 Mo O3 93.6(7) . .
O1 Mo O3 133.9(8) . .
O17 Mo O3 97.6(8) . 3_567
O2 Mo O3 157.4(7) . 3_567
O1 Mo O3 77.2(7) . 3_567
O3 Mo O3 70.7(7) . 3_567
O17 Mo U2 103.3(6) . .
O2 Mo U2 143.0(6) . .
O1 Mo U2 41.4(6) . .
O3 Mo U2 102.7(5) . .
O3 Mo U2 36.0(4) 3_567 .
Mo O1 U3 145.6(9) . 1_455
Mo O1 U2 110.9(8) . .
U3 O1 U2 100.3(5) 1_455 .
Mo O2 U3 142.0(9) . 3_567
Mo O3 Mo 109.3(7) . 3_567
Mo O3 U2 132.8(8) . 3_567
Mo O3 U2 108.7(7) 3_567 3_567
U3 O4 U5 163.3(9) . 1_556
U2 O5 U6 164.5(9) . 1_556
U6 O6 Li1 140.6(17) . .
U2 O7 U1 135.9(8) . 4_576
U2 O7 U4 106.2(6) . 4_476
U1 O7 U4 116.7(6) 4_576 4_476
U4 O8 Li2 178(2) . 4_676
U3 O9 U1 137.3(8) . 4_576
U3 O9 U4 105.9(7) . 4_576
U1 O9 U4 116.4(7) 4_576 4_576
U2 O10 U3 140.2(7) . .
U2 O10 U1 110.6(7) . .
U3 O10 U1 108.6(7) . .
U1 O11 Li1 153.3(16) . .
U1 O12 Li1 175.8(18) . 4_576
U3 O13 U4 142.1(8) . .
U3 O13 U1 111.8(7) . .
U4 O13 U1 106.0(6) . .
Li2 O14 U5 101.9(19) 3_566 .
Li2 O14 U6 112.7(19) 3_566 .
U5 O14 U6 142.0(7) . .
U5 O15 Li1 139.9(17) . .
U5 O15 Li2 97.7(15) . 1_655
Li1 O15 Li2 120(2) . 1_655
U2 O16 U3 130.6(7) . 1_455
U2 O16 U4 115.7(7) . 4_476
U3 O16 U4 113.7(6) 1_455 4_476
Mo O17 Li2 168(2) . .
U2 O18 U4 142.7(8) . 1_455
U2 O18 U1 110.0(7) . .
U4 O18 U1 107.3(6) 1_455 .
U4 O19 Li2 177(2) . 1_655
O11 Li1 O6 113(3) . .
O11 Li1 O15 128(3) . .
O6 Li1 O15 106(2) . .
O11 Li1 O12 98.2(17) . 4_575
O6 Li1 O12 100(2) . 4_575
O15 Li1 O12 108(3) . 4_575
O11 Li1 U5 145(2) . .
O6 Li1 U5 87.2(14) . .
O15 Li1 U5 19.6(8) . .
O12 Li1 U5 106(2) 4_575 .
O11 Li1 U6 132(2) . .
O6 Li1 U6 19.4(9) . .
O15 Li1 U6 87.4(14) . .
O12 Li1 U6 100.1(17) 4_575 .
U5 Li1 U6 68.4(7) . .
O11 Li1 U1 13.1(8) . .
O6 Li1 U1 121(2) . .
O15 Li1 U1 128(2) . .
O12 Li1 U1 86.1(13) 4_575 .
U5 Li1 U1 147.9(14) . .
U6 Li1 U1 140.1(15) . .
O11 Li1 U1 99.3(14) . 4_575
O6 Li1 U1 101.4(17) . 4_575
O15 Li1 U1 106(2) . 4_575
O12 Li1 U1 2.0(8) 4_575 4_575
U5 Li1 U1 103.8(13) . 4_575
U6 Li1 U1 100.5(12) . 4_575
U1 Li1 U1 87.1(8) . 4_575
O8 Li2 O17 162(3) 4_475 .
O8 Li2 O14 95(2) 4_475 3_566
O17 Li2 O14 96(2) . 3_566
O8 Li2 O19 82.2(17) 4_475 1_455
O17 Li2 O19 85.6(19) . 1_455
O14 Li2 O19 175(3) 3_566 1_455
O8 Li2 O15 99(2) 4_475 1_455
O17 Li2 O15 98(2) . 1_455
O14 Li2 O15 74.2(17) 3_566 1_455
O19 Li2 O15 110(3) 1_455 1_455
O8 Li2 U5 99.7(18) 4_475 1_455
O17 Li2 U5 97.9(16) . 1_455
O14 Li2 U5 39.7(11) 3_566 1_455
O19 Li2 U5 145(3) 1_455 1_455
O15 Li2 U5 34.5(8) 1_455 1_455
O8 Li2 U6 98(2) 4_475 .
O17 Li2 U6 83.9(19) . .
O14 Li2 U6 34.5(12) 3_566 .
O19 Li2 U6 142(3) 1_455 .
O15 Li2 U6 107.7(16) 1_455 .
U5 Li2 U6 73.3(10) 1_455 .
O8 Li2 U4 0.8(10) 4_475 4_475
O17 Li2 U4 163(2) . 4_475
O14 Li2 U4 94.6(15) 3_566 4_475
O19 Li2 U4 82.4(13) 1_455 4_475
O15 Li2 U4 97.8(16) 1_455 4_475
U5 Li2 U4 99.1(12) 1_455 4_475
U6 Li2 U4 97.9(12) . 4_475
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
U1 O12 1.790(15) .
U1 O11 1.813(15) .
U1 O9 2.269(18) 4_575
U1 O7 2.273(16) 4_575
U1 O10 2.418(14) .
U1 O13 2.550(16) .
U1 O18 2.609(16) .
U2 O5 1.879(16) .
U2 O18 1.941(16) .
U2 O16 2.127(15) .
U2 O10 2.133(17) .
U2 O7 2.160(16) .
U2 O3 2.272(16) 3_567
U2 O1 2.590(17) .
U3 O4 1.859(15) .
U3 O13 1.929(16) .
U3 O10 2.165(18) .
U3 O16 2.167(16) 1_655
U3 O9 2.218(16) .
U3 O2 2.426(16) 3_567
U3 O1 2.492(19) 1_655
U4 O19 1.781(15) .
U4 O8 1.797(14) .
U4 O16 2.242(14) 4_675
U4 O18 2.392(16) 1_655
U4 O9 2.403(18) 4_575
U4 O13 2.422(16) .
U4 O7 2.459(16) 4_675
U5 O15 1.826(15) .
U5 O15 1.826(15) 3_666
U5 O14 2.083(14) 3_666
U5 O14 2.083(14) .
U5 O4 2.391(15) 1_554
U5 O4 2.391(15) 3_667
U6 O6 1.855(17) .
U6 O6 1.855(17) 3_566
U6 O14 2.117(14) 3_566
U6 O14 2.117(14) .
U6 O5 2.381(16) 3_567
U6 O5 2.381(16) 1_554
Mo O17 1.722(15) .
Mo O2 1.745(16) .
Mo O1 1.819(17) .
Mo O3 1.932(16) .
Mo O3 2.230(16) 3_567
Li1 O12 1.97(4) 4_575
Li2 O8 2.00(4) 4_475
Li2 O14 2.03(5) 3_566
Li2 O19 2.08(5) 1_455
Li2 O15 2.38(6) 1_455
